intermediate phases - ?· intermediate phases ... either congruent or incongruent melting phases....
Post on 20-Aug-2018
Embed Size (px)
Phase DiagramsUnderstanding the BasicsF.C. Campbell, editor
Copyright 2012 ASM InternationalAll rights reserved
Chapter 9Intermediate Phases
PhASe DIAgrAMS are often quite complex, with a number of dif-ferent reactions occurring at different compositions and temperatures. In most cases, the appearance of several reactions in a binary phase diagram is the result of the presence of intermediate phases. These are phases whose chemical compositions are intermediate between the two pure metals, and whose crystalline structures are different from those of the pure metals. The difference in crystalline structure distinguishes intermediate phases from primary solid solutions, which are based on pure metals. Some inter-mediate phases can accurately be called intermetallic compounds, when, like Mg2Pb, they have a fixed simple ratio of the two kinds of atoms. How-ever, many intermediate phases that exist over a range of compositions are considered to be intermediate or secondary solid solutions.
Intermediate phases can be classified based on their melting behavior, either congruent or incongruent melting phases. On heating, an incongru-ent melting phase decomposes into two different phases, usually one solid and one liquid, such as a peritectic transformation. A congruent melting phase melts in the same manner as a pure metal. In this case, the phase diagram is divided into essentially independent sections. In Fig. 9.1, the congruent melting phase divides the lead-magnesium diagram into two separate eutectic reactions that can be analyzed separately. The phase is the intermetallic compound Mg2Pb that has a simple fixed ratio of the two kinds of metal atoms. The details of different types of intermetallic compounds were covered in Chapter 2, Solid Solutions and Phase Trans-formations in this book. Many intermetallic compounds are avoided in alloying because they tend to be hard and brittle.
The copper-zinc phase diagram shown in Fig. 9.2 contains intermedi-ate phases with appreciable ranges of solid solubility. In this diagram, the copper-rich solid solution and the zinc-rich solid solution are the two terminal phases, and the four intermediate phases are , , , and . The copper-zinc system forms the basis for the industrially important brass alloys. As shown in the copper-rich portion of the copper-zinc diagram
5342_ch09_6111.indd 171 3/2/12 12:26:17 PM
172 / Phase DiagramsUnderstanding the Basics
of Fig. 9.3, -copper can dissolve up to 32.5% Zn at the solidus tempera-ture of 900 C (1655 F), the proportion increasing to 39.0% at 455 C (850 F). Although the amount of zinc decreases with further decreases in temperature, diffusion is very sluggish at temperatures below 455 C (850 F), and with ordinary industrial cooling rates, the amount of zinc that can remain in solid solution in copper at room temperature is approximately 39%. When the amount of zinc is increased beyond 39%, the intermedi-ate ordered phase, equivalent to CuZn, will form on slow cooling. This phase is hard at room temperature and has limited ductility but becomes plastic when it changes to the disordered phase above 455 C (850 F). Unlike copper, which is face-centered cubic (fcc) and zinc, which is hex-agonal close-packed (hcp), the phases are body-centered cubic (bcc). The high-temperature phase is disordered, while the lower-temperature phase is ordered (Fig. 9.4). These alloys are easy to machine and hot form but are not very amendable to cold forming, because the phase is brittle at room temperature. There is also a rapid reduction in the impact strength with a simultaneous increase in hardness and tensile strength. The maximum strength is attained at 44% Zn. Further increases in the zinc content beyond 50% causes the phase to form, which is too brittle for engineering alloys.
Fig. 9.1 Compound formation in magnesium-lead system. Source: ref 9.1
5342_ch09_6111.indd 172 3/2/12 12:26:18 PM
Chapter 9: Intermediate Phases / 173
Fig. 9.2 Copper-zinc phase diagram. Source: ref 9.1
Fig. 9.3 Copper-rich section of copper-zinc phase diagram. Source: ref 9.1
Because alloys that contain only the phase are quite soft and ductile at room temperature, the -brasses are very amendable to cold working. however, as a result of the hard, ordered phase, brasses containing both the + phases are rather hard, with a low capacity for cold work. The
5342_ch09_6111.indd 173 3/2/12 12:26:18 PM
174 / Phase DiagramsUnderstanding the Basics
+ brasses are hot worked in the temperature range where transforms . Thus, the -brasses are often referred to as cold work brasses and the + brasses are known as hot work brasses.
9.1 Order-Disorder Transformations
An order-disorder transformation typically occurs on cooling from a disordered solid solution to an ordered phase. During this phase trans-formation, there is a rearrangement of atoms from random site locations in the disordered solution to specific lattice sites in the ordered structure. When atoms periodically arrange themselves into a specific ordered array, they make up what is commonly referred to as a superlattice. Although many alloy systems may contain ordered phases, only select superlattices are discussed in this chapter. Four common superlattice structures and ordered phases that atomically arrange into the corresponding superlattice are listed in Table 9.1. As noted in the table, the superlattice types can be referred to by Strukturbericht symbols (L10, L12, B2, and D03) or by the prototype phase (CuAu I, Cu3Au, FeAl, Fe3Al).
Antiphase Boundaries. Most alloys that form an ordered structure are disordered at higher temperature, which means that atoms are randomly located on lattice sites. On cooling, small ordered areas will nucleate within the disordered phase and begin to grow into ordered domains. These ordered domains can also form by a continuous ordering mechanism, where local atomic rearrangements occur homogeneously throughout the disor-dered phase, creating ordered domains. As the temperature is decreased further, the ordered domains will grow until they impinge on or intersect
Fig. 9.4 Disordered and ordered structures in 50% Cu-50% Zn -brasses. Source: ref 9.1
5342_ch09_6111.indd 174 3/2/12 12:26:18 PM
Chapter 9: Intermediate Phases / 175
each other and form antiphase boundaries (APBs). Antiphase boundaries are boundaries between two ordered domains where the periodicity of the ordered structure in one domain is out of step with the other. This is shown in Fig. 9.5, which is a schematic representing the phase transfor-mation from a disordered structure at elevated temperature to the ordered structure, with APBs located where the domains intersect. The APBs are typically well defined within the structure and can be seen fairly easily using thin-film transmission electron microscopy (TEM).
Long-Range and Short-Range Order. A perfectly ordered structure is one that has the periodic arrangements of atoms throughout the entire crystal, without the presence of any defects. Practically, defects that dis-rupt the atomic sequence are typically found within the crystal lattice. For example, if an aluminum atom replaced an iron atom in the ordered FeAl phase, the structure would be less than perfect. Therefore, a parameter, S,
Table 9.1 Selected superlattice structures and alloy phases that order according to each superlattice
Strukturbericht symbol Prototype phase Base lattice type Phases
L10 CuAu I Face-centered cubic AgTi, AlTi, CoPt, CrPd, CuAu, Cu3Pd, FePd, FePt, hgPd, hgPt, hgTi, hgZr, InMg, MgTl, MnNi, Mn2Pd3, MnPt, NiPt, PbZn, PtZn
L12 Cu3Au Face-centered cubic AgPt3, Ag3Pt, AlCo3, AlNi3, AlZr3, AuCu3 I, Au3Pt, CaPb3, CaSn3, CdPt3, CePb3, CeSn3, CoPt3, Cr2Pt, CuPd, Cu3Au, Cu3Pt, FeNi3, FePt3, Fe3Pt, geNi3, hgTi3, InMg3, LaPb3, LaSn3, MnNi3, MnPt3, Mn3Pt, NaPb3, Ni3Pt, PbPd3, PbPt3, Pt3Sn, Pt3Ti, Pt3Zn, TiZn3
B2 FeAl Body-centered cubic AgCd, AgCe, AgLa, AgLi, AgMg, AlCo, AlCu2Zn, AuCd, AuMg, AuMn, AuZn, BeCo, BeCu, BeNi, CdCe, Cehg, CeMg, CeZn, CoFe, CoTi, CsCl, CuPd, CuZn, CuZn3, FeAl, FeTi, hgLi2Tl, hgMn, InNi, LaMg, LiPb, LiTl, MgPr, MgSr, MgTl, MnPt, NiAl, NiTi, ruTa, TiZn
D03 Fe3Al Simple cubic BiLi3, CeMg3, Cu3Sb, Fe3Al, Fe3Si, Mg3Pr
Source: ref 9.2 as published in ref 9.3
Fig. 9.5 Schematic representation of (a) a disordered solution and (b) an ordered structure with an antiphase boundary (apB) (dashed line) located where the atomic sequence is out of step.
Source: ref 9.3
5342_ch09_6111.indd 175 3/2/12 12:26:19 PM
176 / Phase DiagramsUnderstanding the Basics
was established to quantify the degree of long-range order within a crystal. For binary alloys (alloy A-B), if A atoms occupy the sublattice, and B atoms occupy the sublattice:
S f ff
where fA is the fraction of all A atoms in the alloy, and fA() is the fraction of A atoms that lie on the sublattice. The term fA() can also be described as the probability that an A atom occupies an site. It can be seen from this equation that the degree of long-range order can be quantified, where a completely disordered solution is present when S = 0, and a perfectly ordered structure is present when S = 1.
Long-range order is used to describe the degree of ordering throughout an entire crystal. There is also a degree of ordering, known as short-range ordering, that is associated with a single atom and its nearest neighbors. In a crystal lattice, each atom has first- and second-order nearest neighbors. In an A-B alloy with a random arrangement of atoms (disordered solu-tion), each A atom should have an average number of B nearest neighbors. In an ordered structu